The use of solid supports and ultra-high vacuum conditions for the synthesis of two-dimensional polymers is attractive, as it can enable thorough characterization, often with submolecular resolution, and prevent contamination. However, most on-surface polymerizations are thermally activated, which often leads to high defect densities and relatively small domain sizes. Here, we have obtained a porous two-dimensional polymer that is ordered on the mesoscale by the two-staged topochemical photopolymerization of fluorinated anthracene triptycene (fantrip) monomers on alkane-passivated graphite surfaces under ultra-high vacuum. First, the fantrip monomers self-assemble into highly ordered monolayer structures, where all anthracene moieties adopt a suitable arrangement for photopolymerization. Irradiation with violet light then induces complete covalent crosslinking by [4+4] photocycloaddition to form a two-dimensional polymer, while fully preserving the long-range order of the self-assembled structure. The extent of the polymerization is confirmed by local infrared spectroscopy and scanning tunnelling microscopy characterization, in agreement with density functional theory calculations, which also gives mechanistic insights.
This is a preview of subscription content, access via your institution
Open Access articles citing this article.
Nature Communications Open Access 21 January 2022
Access Nature and 54 other Nature Portfolio journals
Get Nature+, our best-value online-access subscription
$29.99 / 30 days
cancel any time
Subscribe to this journal
Receive 12 print issues and online access
$259.00 per year
only $21.58 per issue
Rent or buy this article
Prices vary by article type
Prices may be subject to local taxes which are calculated during checkout
Perepichka, D. F. & Rosei, F. Extending polymer conjugation into the second dimension. Science 323, 216–217 (2009).
Sakamoto, J., van Heijst, J., Lukin, O. & Schlüter, A. D. Two-dimensional polymers: just a dream of synthetic chemists? Angew. Chem. Int. Ed. 48, 1030–1069 (2009).
Celebi, K. et al. Ultimate permeation across atomically thin porous graphene. Science 344, 289–292 (2014).
Zhuang, X. D., Mai, Y. Y., Wu, D. Q., Zhang, F. & Feng, X. L. Two-dimensional soft nanomaterials: a fascinating world of materials. Adv. Mater. 27, 403–427 (2015).
Ferrari, A. C. et al. Science and technology roadmap for graphene, related two-dimensional crystals, and hybrid systems. Nanoscale 7, 4598–4810 (2015).
Lackinger, M. On-surface polymerization—a versatile synthetic route to two-dimensional polymers. Polym. Int. 64, 1073–1078 (2015).
Payamyar, P., King, B. T., Ottinger, H. C. & Schlüter, A. D. Two-dimensional polymers: concepts and perspectives. Chem. Commun. 52, 18–34 (2016).
Wang, W. & Schlüter, A. D. Synthetic 2D polymers: a critical perspective and a look into the future. Macromol. Rapid Commun. 40, e1800719 (2019).
Colson, J. W. & Dichtel, W. R. Rationally synthesized two-dimensional polymers. Nat. Chem. 5, 453–465 (2013).
Moreno, C. et al. Bottom-up synthesis of multifunctional nanoporous graphene. Science 360, 199–203 (2018).
Galeotti, G. et al. Synthesis of mesoscale ordered two-dimensional π-conjugated polymers with semiconducting properties. Nat. Mater. 19, 874–880 (2020).
Kissel, P., Murray, D. J., Wulftange, W. J., Catalano, V. J. & King, B. T. A nanoporous two-dimensional polymer by single-crystal-to-single-crystal photopolymerization. Nat. Chem. 6, 774–778 (2014).
Kory, M. J. et al. Gram-scale synthesis of two-dimensional polymer crystals and their structure analysis by X-ray diffraction. Nat. Chem. 6, 779–784 (2014).
Lange, R. Z., Hofer, G., Weber, T. & Schlüter, A. D. A two-dimensional polymer synthesized through topochemical [2+2]-cycloaddition on the multigram scale. J. Am. Chem. Soc. 139, 2053–2059 (2017).
Payamyar, P. et al. Synthesis of a covalent monolayer sheet by photochemical anthracene dimerization at the air/water interface and its mechanical characterization by AFM indentation. Adv. Mater. 26, 2052–2058 (2014).
Murray, D. J. et al. Large area synthesis of a nanoporous two-dimensional polymer at the air/water interface. J. Am. Chem. Soc. 137, 3450–3453 (2015).
Müller, V. et al. Structural characterization of a covalent monolayer sheet obtained by two-dimensional polymerization at an air/water interface. Angew. Chem. Int. Ed. 56, 15262–15266 (2017).
Müller, V. et al. A two-dimensional polymer synthesized at the air/water interface. Angew. Chem. Int. Ed. 57, 10584–10588 (2018).
Bauer, T. et al. Synthesis of free-standing, monolayered organometallic sheets at the air/water interface. Angew. Chem. Int. Ed. 50, 7879–7884 (2011).
Kambe, T. et al. π-Conjugated nickel bis(dithiolene) complex nanosheet. J. Am. Chem. Soc. 135, 2462–2465 (2013).
Dai, W. Y. et al. Synthesis of a two-dimensional covalent organic monolayer through dynamic imine chemistry at the air/water interface. Angew. Chem. Int. Ed. 55, 213–217 (2016).
Liu, K. J. et al. On-water surface synthesis of crystalline, few-layer two-dimensional polymers assisted by surfactant monolayers. Nat. Chem. 11, 994–1000 (2019).
Beyer, H., Kory, M. J., Hofer, G., Stemmer, A. & Schlüter, A. D. Exfoliation of two-dimensional polymer single crystals into thin sheets and investigations of their surface structure by high-resolution atomic force microscopy. Nanoscale 9, 9481–9490 (2017).
Bieri, M. et al. Porous graphenes: two-dimensional polymer synthesis with atomic precision. Chem. Commun. 2009, 6919–6921 (2009).
Klappenberger, F. et al. On-surface synthesis of carbon-based scaffolds and nanomaterials using terminal alkynes. Acc. Chem. Res. 48, 2140–2150 (2015).
Fan, Q. T., Gottfried, J. M. & Zhu, J. F. Surface-catalyzed C–C covalent coupling strategies toward the synthesis of low-dimensional carbon-based nanostructures. Acc. Chem. Res. 48, 2484–2494 (2015).
Dong, L., Liu, P. N. & Lin, N. Surface-activated coupling reactions confined on a surface. Acc. Chem. Res. 48, 2765–2774 (2015).
Talirz, L., Ruffieux, P. & Fasel, R. On-surface synthesis of atomically precise graphene nanoribbons. Adv. Mater. 28, 6222–6231 (2016).
Lackinger, M. Surface-assisted Ullmann coupling. Chem. Commun. 53, 7872–7885 (2017).
Clair, S. & de Oteyza, D. G. Controlling a chemical coupling reaction on a surface: tools and strategies for on-surface synthesis. Chem. Rev. 119, 4717–4776 (2019).
Grill, L. & Hecht, S. Covalent on-surface polymerization. Nat. Chem. 12, 115–130 (2020).
Eichhorn, J. et al. On-surface Ullmann coupling: the influence of kinetic reaction parameters on the morphology and quality of covalent networks. ACS Nano 8, 7880–7889 (2014).
Gao, H. Y. et al. Glaser coupling at metal surfaces. Angew. Chem. Int. Ed. 52, 4024–4028 (2013).
Wiengarten, A. et al. Surface-assisted dehydrogenative homocoupling of porphine molecules. J. Am. Chem. Soc. 136, 9346–9354 (2014).
Mali, K. S., Pearce, N., De Feyter, S. & Champness, N. R. Frontiers of supramolecular chemistry at solid surfaces. Chem. Soc. Rev. 46, 2520–2542 (2017).
Bhola, R. et al. A two-dimensional polymer from the anthracene dimer and triptycene motifs. J. Am. Chem. Soc. 135, 14134–14141 (2013).
Schmidt, G. M. J. Photodimerization in the solid state. Pure Appl. Chem. 27, 647–678 (1971).
Wolf, M. & Tegeder, P. Reversible molecular switching at a metal surface: a case study of tetra-tert-butyl-azobenzene on Au(111). Surf. Sci. 603, 1506–1517 (2009).
Gao, H. Y. et al. Photochemical glaser coupling at metal surfaces. J. Phys. Chem. C 118, 6272–6277 (2014).
Shen, Q. et al. Self-assembled two-dimensional nanoporous molecular arrays and photoinduced polymerization of 4-bromo-4'-hydroxybiphenyl on Ag(111). J. Chem. Phys. 142, 101902 (2015).
Basagni, A. et al. On-surface photo-dissociation of C–Br bonds: towards room temperature Ullmann coupling. Chem. Commun. 51, 12593–12596 (2015).
Guo, H., Saalfrank, P. & Seideman, T. Theory of photoinduced surface reactions of admolecules. Prog. Surf. Sci. 62, 239–303 (1999).
Miura, A. et al. Light- and STM-tip-induced formation of one-dimensional and two-dimensional organic nanostructures. Langmuir 19, 6474–6482 (2003).
Colazzo, L., Sedona, F., Moretto, A., Casarin, M. & Sambi, M. Metal-free on-surface photochemical homocoupling of terminal alkynes. J. Am. Chem. Soc. 138, 10151–10156 (2016).
Tersoff, J. & Hamann, D. R. Theory of the scanning tunneling microscope. Phys. Rev. B 31, 805–813 (1985).
Hofer, G., Grieder, F., Kroger, M., Schlüter, A. D. & Weber, T. Unraveling two-dimensional polymerization in the single crystal. J. Appl. Crystallogr. 51, 481–497 (2018).
Meyer, J. C. et al. Direct imaging of lattice atoms and topological defects in graphene membranes. Nano Lett. 8, 3582–3586 (2008).
Sahabudeen, H. et al. Wafer-sized multifunctional polyimine-based two-dimensional conjugated polymers with high mechanical stiffness. Nat. Commun. 7, 13461 (2016).
Teyssandier, J., De Feyter, S. & Mali, K. S. Host–guest chemistry in two-dimensional supramolecular networks. Chem. Commun. 52, 11465–11487 (2016).
Kissel, P. et al. A two-dimensional polymer prepared by organic synthesis. Nat. Chem. 4, 287–291 (2012).
Servalli, M., Trapp, N., Wörle, M. & Klärner, F. G. Anthraphane: an anthracene-based, propeller-shaped D3h-symmetric hydrocarbon cyclophane and its layered single crystal structures. J. Org. Chem. 81, 2572–2580 (2016).
Uejima, M., Sato, T., Tanaka, K. & Kaji, H. Enhancement of fluorescence in anthracene by chlorination: vibronic coupling and transition dipole moment density analysis. Chem. Phys. 430, 47–55 (2014).
Nečas, D. & Klapetek, P. Gwyddion: an open-source software for SPM data analysis. Cent. Eur. J. Phys. 10, 181–188 (2012).
Kresse, G. & Furthmüller, J. Efficient iterative schemes for ab initio total-energy calculations using a plane-wave basis set. Phys. Rev. B 54, 11169–11186 (1996).
Blöchl, P. E. Projector augmented-wave method. Phys. Rev. B 50, 17953–17979 (1994).
Dion, M., Rydberg, H., Schröder, E., Langreth, D. C. & Lundqvist, B. I. Van der Waals density functional for general geometries. Phys. Rev. Lett. 92, 109902 (2004).
Hamada, I. van der Waals density functional made accurate. Phys. Rev. B 89, 121103 (2014).
Henkelman, G., Uberuaga, B. P. & Jonsson, H. A climbing image nudged elastic band method for finding saddle points and minimum energy paths. J. Chem. Phys. 113, 9901–9904 (2000).
Kaestner, J. & Sherwood, P. Superlinearly converging dimer method for transition state search. J. Chem. Phys. 128, 014106 (2008).
Porezag, D. & Pederson, M. R. Infrared intensities and Raman-scattering activities within density-functional theory. Phys. Rev. B 54, 7830–7836 (1996).
Tersoff, J. & Hamann, D. R. Theory and application for the scanning tunneling microscope. Phys. Rev. Lett. 50, 1998–2001 (1983).
Lorente, N. & Persson, M. Theoretical aspects of tunneling-current-induced bond excitation and breaking at surfaces. Faraday Discuss. 117, 277–290 (2000).
VASP TDM code (GitHub, 8 November 2019); https://github.com/QijingZheng/VASP_TDM
The Nanosystems-Initiative-Munich (M.L. and W.M.H.) Cluster of Excellence and the Deutsche Forschungsgemeinschaft (grant no. LA 1842/9-1, M.L.) are gratefully acknowledged for funding. J.B. and J.R. acknowledge funding from the Swedish Research Council and the Swedish Government Strategic Research Area in Materials Science on Functional Materials at Linköping University (Faculty Grant SFO-Mat-LiU no. 2009 00971, received by Linköping University). J.R. also acknowledges funding from the Knut and Alice Wallenberg Foundation. Computational resources were allocated by the Swedish National Infrastructure for Computing and carried out at the National Supercomputer Centre, Sweden.
The authors declare no competing interests.
Peer review information Nature Chemistry thanks the anonymous reviewers for their contribution to the peer review of this work.
Publisher’s note Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
DFT-optimized structures of single fantrip molecules with their anthracene blades adsorbed a, on edge (−1.11 eV) vs. b, parallel (−1.89 eV) on pristine bilayer graphene; as well as c, on edge (−0.93 eV) vs. d, parallel (−1.48 eV) on alkane-passivated bilayer graphene. Top and side views are shown in the upper and lower row, respectively. Adsorption energies with respect to single geometry-optimized fantrip molecules in vacuum are stated in parenthesis. The hexacosane monolayer was modelled as densely packed monolayer of infinite polyethylene strands aligned along a graphite high symmetry direction as experimentally observed for hexacosane (Supplementary Fig. 2). Atom colour code: F, green; C, grey; H, light grey.
First, fantrip was deposited onto hexacosane-passivated graphite and heated at 80 °C to afford self-assembly of exclusively the hexagonal structure. a, STM image of the as prepared sample, that is without further illumination. b, STM image of a sample prepared as in a, but illuminated with laser light to afford a fully cross-linked 2DP. Then both samples were heated to 150 °C for 20 min under identical conditions. c, Line-profile as indicated in b. d, STM image of the non-illuminated sample acquired after heating. The original hexagonal self-assembly was converted into the densely packed fantrip structure as observed for direct deposition onto graphite (Fig. 2a of main manuscript and Supplementary Fig. 1). Even though the ordering has improved, a unit cell can still not be assigned. The conversion is explained by reorganization of fantrip as a consequence of desorption of the hexacosane buffer layer. e, STM image of the illuminated sample acquired after heating, confirming the continued existence of the 2DP. f, Line-profile as indicated in e. The hexacosane monolayer was mostly desorbed, but remnants are still visible at the 2DP boundary. This allows measuring apparent heights of the 2DP of 0.52 nm with regards to graphite and of 0.20 nm with regards to hexacosane, suggesting that the hexacosane monolayer may still be present underneath the 2DP. (Tunneling parameters and scale bars: a −3.0 V, 3 pA, 10 nm; b −3.0 V, 4 pA, 30 nm; d −3.3 V, 3 pA, 10 nm; e -3.0 V, 4 pA, 40 nm).
To evaluate the temperature dependence of the photopolymerization yield, supramolecular fantrip structures on hexacosane-passivated graphite were illuminated with laser light for a similar duration of 4 h while maintaining constant temperatures of the sample environment in a range between 280 K and 310 K. To this end, samples were loaded into the STM for illumination. Constant temperatures were maintained for the cryostat to which the instrument is mounted by simultaneously cooling with liquid nitrogen and feedback controlled counter heating. Accordingly, stated temperatures do not directly correspond to surface temperatures, which lie well above. Representative STM images acquired for cryostat temperatures during illumination of 280 K (a), 290 K (b), 300 K (c) and 310 K (d). e, Plot of the polymerized fraction as obtained from statistical analysis of STM data vs. cryostat temperature. Red dots represent data points corresponding to the mean value obtained from four 25 × 25 nm² STM images; error bars denote standard deviations of the experimental means; the blue line serves as guide to the eye. The graph corroborates increasing degrees of polymerization for increasing surface temperatures around room temperature. (Tunneling parameters: a −3.0 V, 3 pA; b -2.8 V, 3 pA; c -3.0 V, 3 pA; d -2.8 V, 3 pA; all scale bars: 20 nm).
a, Overview STM image of a nearly completely polymerized sample, showing two distinct types of bright features on top; Features with lower apparent height (red circle) are more abundant. These appear with fairly uniform contrast, whereas the higher appearing features (green circle) show a broader size and shape variation. We tentatively attribute the latter to fantrip molecules that became relocated onto the 2DP during the polymerization. The size and shape variability suggests that these features could be comprised of more than one fantrip monomer. b Close-up STM image of a 2DP, where covalent linkages appear as round protrusions. Several brighter appearing features are accumulated in the lower right corner that correspond to the feature highlighted by the red circle in (a). Both their positioning at the network vertices and their uniform internal contrast suggest that these features correspond to non-polymerized fantrip monomers or individual anthracene blades of monomers within the network. (Tunneling parameters and scale bars: a -2.8 V, 3 pA, 10 nm; b -2.8 V, 3 pA, 3 nm).
The regions of interest for locally acquiring IR spectra by nano-FTIR were identified in previously recorded AFM topographies of supramolecular networks (a) and 2DP (b), both on hexacosane-passivated graphite. The AFM images were acquired in tapping mode. Crosses indicate the positions, where IR spectra were acquired (colours correspond to Fig. 6 of main manuscript) from two independent domains for each. These AFM images also indicate lateral domain extensions in the order of 500 nm. (a 150 px × 150 px; b 100 px × 100 px, 10 ms per pixel, scale bars: 500 nm).
ToF-SIMS data (counts vs. ion mass in AMU, positive ions detected) acquired from self-assembled fantrip monolayer on hexacosane-passivated graphite (as in Fig. 2b of main manuscript) (a) and similarly prepared sample after illumination under conditions that afford complete photopolymerization (as in Fig. 5 of main manuscript) (b); Note the logarithmic scale on the vertical axis.
The temperature dependent photopolymerization experiments (Extended Data Fig. 3) also indicated a lower density of Stone-Wales defects. This overview STM image was acquired from a fully polymerized 2DP that was prepared by 14 h illumination with the sample loaded into the STM and the cryostat temperature held constant at 330 K. While for room temperature polymerization ~10 Stone-Wales defects were observed per 100 × 100 nm² of the 2DP (Fig. 5 of main manuscript), this image indicates a lower density with only 2-3 Stone-Wales defects per 100 × 100 nm² of the 2DP. The inset shows the corresponding FFT, corroborating a hexagonal symmetry and the absence of orientational disorder. (Tunneling parameters and scale bars: a -2.8 V, 3 pA, 50 nm; inset 1 nm-1).
Supplementary Figs. 1–26 and synthesis protocol for fantrip monomers.
Source data for Supplementary Figs. 19 and 20. Calculated energies per unit cell versus lattice parameters.
Zip file summarizing all coordinates of DFT-calculated structures as *.xyz files.
About this article
Cite this article
Grossmann, L., King, B.T., Reichlmaier, S. et al. On-surface photopolymerization of two-dimensional polymers ordered on the mesoscale. Nat. Chem. 13, 730–736 (2021). https://doi.org/10.1038/s41557-021-00709-y
This article is cited by
Nature Reviews Methods Primers (2023)
Nature Communications (2022)
Fast water transport and molecular sieving through ultrathin ordered conjugated-polymer-framework membranes
Nature Materials (2022)
On-water surface synthesis of charged two-dimensional polymer single crystals via the irreversible Katritzky reaction
Nature Synthesis (2021)